Rietveld quality parameters refinement and crystal parameters to K
In a normal metallic conductor the electrical resistivity decreases until it reaches a lower limit (˃0) when heat energy is removed from the system. In these materials electrons are scattered by the lattice and obey Fermi-Dirac statistics . The behaviour of a gas of identical particles at low temperature depends on the spin of the particle. Fermions are formed by half-integral spin, and obey Pauli’s exclusion principle, wherein two of them cannot have the same quantum numbers . However many metals, alloys and compounds exhibit the electrical resistivity dropping suddenly to zero and exclude magnetic flux completely when cooled down to a sufficiently low temperature . This phenomenon is known as superconductivity. It was observed first by Kamerlingh Onnes in 1911, a couple of years after the first liquefied helium . At a critical temperature
It is interesting to note that when a superconductor is cooled below its critical temperature its electronic properties change appreciably, but its crystalline structure remains the same, as revealed by X-ray or neutron diffraction studies. Furthermore, the formation mechanism of photons that depends on the thermal vibrations of the atoms remains the same in the superconducting phase as in the normal state. This means that superconductivity is not associated with any remarkable change in the crystalline structure of the specimens. However, although superconductivity is not a property of particular atoms, it does depend strongly on their arrangement. The conduction electrons themselves must be responsible for the superconducting behaviour. A feature that illustrates an important characteristic of these superconducting electrons is that the transition from the normal to the superconducting state is very sharp [3,4]. This could only happen if the electrons in a superconductor become condensed into a coherent, ordered state, which extends over long distances compared to the distances between the atoms. A superconducting state is more ordered than the normal state in a metal. This means that it has a lower entropy, the parameter that measures the amount of disorder in a system. In an analogous way, the entropy of a solid is lower than that of a liquid at the same temperature; solids are more ordered than liquids. So, when a material turns to a superconducting state, the superconducting electrons must be condensed into an ordered state compared to normal electrons.
But what happens if, in a material, the electronic interaction leads to the formation of Cooper pairs but in a disordered state? If this were so then any local variations from collective action between the electrons would broaden the transition over a much wider temperature range or transition could not be noticed. Thus, despite the existence of the Cooper pairs, the state formed would be unconventional metallic but not superconductor. Due to the existence of bosonic particles in the crossover from weak coupling Bardeen-Cooper-Schrieffer (BCS) pairing to a Bose-Einstein condensate (BEC) of tightly bound pairs, this unconventional metallic phase is conveniently called Bose metal [5,6]. The Bose metal has been characterized as a system without long-range order. This new state of the matter has attracted a lot of attention over the past decades due to occurrence of a metal-insulator transition in low dimensional systems [5,6]. Experiments have shown that this transition can be induced by disorder or by applying external magnetic field. When a sufficiently high magnetic field is applied in the material the Cooper pairs are completely localized turning its electrical conductivity to zero and leading to an insulating state. Within this framework a scale law was proposed to identify a Bose metal-insulator transition (BMIT). So, this transition can be analysed in terms of two-parameter scaling, as follows:
where is the electrical resistance and is the temperature. , and are critical exponents, and the deviation of the variable parameter (magnetic field) from the critical values . is the critical magnetic field where the BMIT occurs. Such a transition has been recently observed in semimetals as graphite and bismuth , and also in the quasi one-dimensional Li0.9Mo6O17 . Theoretical analysis has suggested that the BMIT in graphite is associated with the transition between Bose metal and excitonic insulator state, whereas in Li0.9Mo6O17 this transition is discussed in terms of localized bosons in a low dimensional system, which could be related to the Luttinger liquid (LL) state.
Another interesting subject to consider is that superconductivity and magnetism are two different ordered states into which substances can condense at low temperatures, and in general these states are opposite to each other . It has generally been believed that the conduction of electrons in a metal cannot be both ferromagnetically ordered and superconducting. In conventional superconductors, local magnetic moments break up the spin singlet Cooper pairs, and hence strongly suppress superconductivity, an effect known as pair-breaking [3,4]. However, since the 1970s several studies on the interplay between superconductivity and magnetism have arisen in the scientific community. Namely, a coexistence between ferromagnetism and Bose metal state has been demonstrated for both highly oriented pyrolitic graphite and graphite sulphur composites . Actually, the authors’ assumed the observation of metal-insulator crossover in both cases might be related to a Bose metal-insulator transition .
This chapter will report results about recent studies on the K
xMoO2-δ crystalline structure
Polycrystalline samples of K
Figure 1 shows the x-ray diffraction patterns of K
Diffractograms of all samples with
For x ≥ 0.3 a second phase appears related to the precursor K2MoO4. Its x-ray diffractogram is shown in figure 1. The existence of impurity in this specimen means that the solubility limit was reached.
In figure 2 is shown the variation of lattice parameters as a function of the K contents (
With increasing the amount of K one can observe a slight increase in unit cell volume, which is caused by the insertion of K in the crystalline lattice of MoO2. For
To expand the knowledge about the physical properties of the K
1.2. Interplay between superconductivity and ferromagnetism in K0.05MoO2
Magnetization curves as a function of the temperature measured in K0.05MoO2-δ sample with H = 10 and 200 Oe are shown in figure 3 performed under zero field cooled (ZFC) and field cooled (FC) regimes.
To study in greater detail the relationship between the ferromagnetism and superconductivity several loops of magnetization as a function of applied magnetic field was obtained above and below T
Hysteresis curves were obtained with applied magnetic field ranging from 0 to 10 kOe at a temperature of 2 K, as shown in Figure 4 (a). It was observed that for values of applied magnetic field up to 1 kOe, the magnetization curve is almost linear as a function of applied magnetic field and is reversible (blue curve) due to the Meissner effect. This result allows one to estimate the lower critical field (H
In the inset of the figure 4 (a) is shown the M(H) at 20 K. We can observe clearly a ferromagnetic ordering very similar to that observed in magnetic superconductors such as RuSr2GdCu2O8 . In the figure 4 (b) is displayed the continuous disappearance of superconductivity when the temperature is increasing. At 9 K the superconductivity almost disappears, leaving only a weak positive magnetic component.
Figure 5 shows magnetization curves as a function of temperature for several samples with different starting compositions. The superconducting critical temperature of each sample is indicated by arrows on the figure.
The inset shows the variation in superconducting critical temperature (T
1.3. Unconventional metallic behaviour
Figure 6 shows the electrical resistance as a function of temperature below 80 K for K0.05MoO2-δ.
The electrical resistance temperature dependence for K0.05MoO2 sample shown in figure 6 exhibits a anomalous metallic behaviour. The blue line is the best fit using the power law such as R(T) = R0 + CTα. The anomalous exponent (α) indicated for the electrical resistance as a function of temperature is the best value found by the fit obtained by the method of least squares. This value of α suggests that the one-dimensional conduction mechanism is described by Luttinger liquid theory, with attractive interaction between electrons [8,12-13]. Furthermore, this result confirms the α ~ 0.5 that has also been observed for several another samples of this system , showing that the anomalous metallic behaviour is characteristic of this material.
The inset of figure 6 shows the core level photoemission spectroscopy for MoO2 and K0.05MoO2-δ. The Mo 3p spectrum of the undoped sample shows two main structures associated with the Mo 3p1/2 and Mo 3p3/2 core levels, which are split due to spin-orbit effects. In the 3p3/2 region, the peak around 395.5 eV is assigned to Mo4+ (4d2) states, but there is also a very small Mo3+ (4d3) contribution at about 393.4 eV. The later can be associated with the covalent Mo-O bond character, which is also supported by the relatively small charge transfer satellite, at around 425 eV. Nevertheless, a small oxygen deficiency in MoO2 cannot be ruled out, as well. In the 3p1/2 region, the corresponding binding energies of the Mo4+ and Mo3+ states are 413.0 and 410.9 eV, respectively. The spectrum of the potassium-doped sample shows a new structure at 376 eV, assigned to the K 2s core level. More importantly, the peaks due to the Mo3+ states in the Mo 3p core level increase and become more prominent. This relative increase indicates that the potassium ions, when incorporated into the MoO2 structure, are effectively doping the Mo 4d band with electrons, from a nominal 4d2 to 4d3. The extra charge introduced in the Mo 4d band by the potassium ions would lead to an effective magnetic moment and might be the origin of magnetism in this material. A similar effect, namely, extra charge induced by the presence of ligand vacancies, was reported as the origin of ferromagnetism in other oxides with nonmagnetic ions. Similarly the electrical behaviour of the K
1.4. Bose-metal insulator transition
With the goal of increasing the understanding of the physical properties of K
Figure 7 shows the electrical resistance as a function of temperature in a zero magnetic applied field as well as in 7 T. The results show an anomalous metallic behaviour at zero applied field. Under the applied magnetic field the electrical resistance changes to higher values indicating a positive magnetoresistance. At zero magnetic field one can observe an anomalous behaviour, in which the electrical resistance decreases as the temperature decreases. As already discussed, this behaviour differs from conventional metal-like behaviour in which the electrical resistance should reach a saturation state at low temperatures.
It is important to note in figure 7 that the anomalous metallic behaviour disappears at very low temperatures (
The critical magnetic field where the Bose metal-insulator transition occurs is better observed by the crossover in the isotherms shown in the Figure 8.
For applied magnetic field lower than the critical value (HC = 5.59 T), the system behaves in the classical model of magnetoresistance as in metallic systems, expressed by
To better characterize the transition from a metal to an insulating state induced by a applied magnetic field, the scaling theory proposed by Das and Doniach  was used. This theory implies the existence of Cooper pairs tightly bound and without long-range order, thus featuring a metallic state at absolute zero (Bose metal). Within this context, these authors proposed a scaling law used to characterize the transition from Bose metal to insulator based on two scaling parameters In the inset the result of this scaling to a critical field HC = 5.59 T and critical exponent are shown.
The deviation of the Fermi liquid behaviour and a perfect correlation between the magnetoresistance data with the model proposed by Das and Doniach  suggests that, at low temperatures and zero applied magnetic field, the K0.05MoO2-δ compound shows the expected for a Bose metal. In this context one may suggest a possible correlation between the unconventional metallic behaviour observed in the curves R(T) below ~70 K with the existence of Cooper pairs tightly bounded without long-range order. This seems to corroborate with the observation of superconductivity in the KxMoO2-δ system [10-11,15].
This chapter reported the influence of defects in the crystalline structure on the properties of K-doped MoO2. Potassium doping leads to superconductivity with critical temperatures up to 10 K and electrical resistance measurements displayed an anomalous behaviour below the temperature showing the manifestation of magnetism (T < 70 K). The study of the anomalies in the electrical behaviour provided important conclusions, such as the temperature dependence of the electrical resistance as described by a power law of the type R(T) = R0 + CTα, where anomalous exponent (α) is found to be near 0.5. This value of α described by the theory of Luttinger liquid (LL) suggests a mechanism for one-dimensional metallic conduction. Furthermore, the LL theory suggests that the interaction between the conduction electrons is attractive to positive α and smaller than one. Under an applied magnetic field the electrical resistance changes to higher values indicating positive magnetoresistance. This behaviour is very similar to a Bose metal-insulator transition. This behaviour was interpreted according to the scaling theory proposed by Das and Doniach. This theory implies the existence of Cooper pairs tightly bound without long-range order, thus featuring a metallic state at absolute zero (Bose metal). This seems to agree with that observed by the LL theory and with the existence of superconductivity in the KxMoO2-δ system.
This material was based upon work supported by the FAPESP (2010/06637-2 and 2009/54001-2) and CNPq (08162/2013-7). J. J. Neumeier, J. B. Leão, R. J. O. Mossanek, and J. A. O. Aguiar are acknowledged for helping with several measurements and previous discussions.
Kittel, C. Introduction to solid state physics, 8th Ed., p. 136 and 277 (Wiley, New York, 2005).
Kamerlingh Onnes, H. Commun. Phys. Lab. Univ. Leiden. Suppl. 29 (Nova York, 1911).
Bardeen, J., Cooper, L. N., and Schriffer, J. R. Microscopic theory of superconductivity. Phys. Rev., 106(1):162–164, Apr 1957.
Bardeen, J., Cooper, L. N., and Schriffer, J. R. Theory of superconductivity. Phys. Rev., 108(5):1175–1204, Dec 1957.
Das, D. and Doniach, S. Bose metal: Gauge-field fluctuations and scaling for field-tuned quantum phase transitions Phys. Rev. B 64, 134511 (2001).
Phillips, P. and Dalidovich, D. The elusive Bose metal. Science 302, 243 (2003).
Kopelevich, Y., Medina Pantoja, J. C., da Silva, R. R., and Moehlecke, S. Universal magnetic-field-driven metal-insulator-metal transformations in graphite and bismuth. Phys. Rev. B 73, 165128 (2006).
dos Santos, C. A. M., da Luz, M. S., Yu, Yi-Kuo, Neumeier, J. J., Moreno, J., and White, B. D., Electrical transport in single-crystalline Li0.9Mo6O17: A two-band Luttinger liquid exhibiting Bose metal behavior. Phys. Rev. B 77, 193106 (2008).
Kopelevich, Y. Esquinazi, P. Torres, J. H. S., Moehlecke, S. Ferromagnetic and superconducting like behavior of Graphite. J. Low Temp. Phys. 119, 691-702 (2000).
Alves, L. M. S., dos Santos, C. A. M., Benaion, S. S., Machado A. J. S., de Lima B. S., Neumeier, J. J., Marques, M. D. R., Albino Aguiar, J., Mossanek, R. J. O., and Abbate, M. Superconductivity and magnetism in the KxMoO2-δ. J. Appl. Phys. 112, 073923 (2012).
Alves, L. M. S., Damasceno, V. I., dos Santos, C. A. M., Bortolozo, A. D., Suzuki, P. A., Izario Filho, H. J., Machado, A. J. S., and Fisk, Z. Unconventional metallic behavior and superconductivity in the K-Mo-O system. Phys. Rev. B 81, 174532 (2010).
Ogata, M., Anderson, P. W. Transport properties in the Tomonaga-Luttinger liquid. Phys. Rev. Letters 70, 3087 (1993).
Pereira, R. G. Transport in ordered one-dimensional systems. Campinas: UNICAMP, 2004. 134p. Dissertation (Master in Physics) - Universidade Estadual de Campinas, Instituto de Física Gleb Wataghin, Campinas, São Paulo, 2004.
Bernhard, C., Tallon, J. L., Niedermayer, Ch., Blasius, Th., Golnik, A., Brücher, E., Kremer, R. K., Noakes, D. R., Stronach, C. E., and Ansaldo, E. J. Coexistence of ferromagnetism and superconductivity in the hybrid ruthenate-cuprate compound RuSr2GdCu2O8 studied by muon spin rotation and dc magnetization. Phys. Rev. B 59, 14099-14107 (1999).
Parker, D., Idrobo, J. C., Cantoni, C., and Sefat, A. S. Evidence for superconductivity at TC = 12 K in oxygen-deficient MoO2−δ and properties of molybdenum arsenide and oxide binaries. Phys. Rev. B 90, 054505 (2014).
Alves, L. M. S. Unconventional electrical behavior in the KxMoO2-δ. 2010. 68 p. Dissertation (Master of Science) – Escola de Engenharia de Lorena, Universidade de São Paulo, Lorena-SP, Brazil, 2010.
Alves, L. M. S., de Lima, B. S., da Luz, M. S.,dos Santos, C. A. M., Neumeier, J. J., and Yu, Yi-Kuo. A magnetic field tuned metal-insulator transition in unconventional metallic K-doped MoO2. To be published.
Danner, G. M.; Chaikin, P. M. Non-fermi-liquid behavior in transport in (TMTSF)2PF6. Phys. Rev. Letters 75, 4690, 1995.